Page:United States Statutes at Large Volume 116 Part 4.djvu/782

 116 STAT. 3210 PROCLAMATION 7529-MAR. 5, 2002 ANNEX (continued) 21 thickness of 1.20 mm, thickness tolerance r 0.09 mm, width tolerance; 0.2mm. tensile strength 45.9 - 64.2 kg/mnv, yield point 31.6 -36.7 kg/mm-, permeability 450 - 630 (at the magnetic force of 0.35 Oc, according to JIS C 2550), with coating weight of 20 g/mnv" (minimum 17 g/mm', maximum 26 g/mm'; approx. thickness 3 pm); or (F) electrogalvanized flat-rolled products (provided for in subheadings 7225.91.00 or 7226.93.00), annealed, containing from 0.0020 percent to 0.0035 percent by weight of boron, from 0.03 percent to 0.6 percent carbon, having a Rockwell hardness from 45 to 60 and a thickness over 0.312 mm but not over 0.38 mm; (xl) corrosion-resistant products designated as X-176, as described below: (A) electrogalvanized flat-rolled products, whether or not including chromate or a chromate-free coating, with the following specifications: tensile strength 45 - 49 kg/mm", yield point 33 - 37 kg/mm', magnetic properties 450p or more, zinc-nickel alloy electroplating, coating weights of zinc 17 g/m' minimum and if applicable chromium 20 - 60 mg/m^ and thickness tolerance +/- 5 percent; having the following chemical composition (in percent by weight): carbon 0.07 maximum, silicon 2.0 maximum, manganese 2.0 maximum, phosphorus 0.15 maximum and sulfur 0.02 maximum; (B) electrogalvanized flat-rolled products, whether or not including chromate or a chromate-free coating, with the following specifications: tensile strength 45 - 49 kg/mm-, yield point 33 - 37 kg/mm-, magnetic properties 450|J or more, zinc-nickel alloy electroplating, coating weights of zinc 17 g/m' minimum and if applicable special chromate treatment with a thickness of film of 0.2 - 0.8 gm and thickness tolerance +/- 5 percent; having the following chemical composition (in percent by weight): carbon 0.07 maximum, silicon 2.0 maximum, manganese 2.0 maximum, phosphorus 0.15 maximum and sulfur 0.02 maximum; (C) high strength electrolytic zinc-coated silicon steel flat-rolled products, whether or not including a chromate or chromate-free coating, with the following specifications: thickness 1.20 mm, thickness tolerance +/-60 pm, width tolerance -0/+7 mm, tensile strength 41 - 45 kg/mm^, yield point 26 - 30 kg/mm^ magnetic properties of permeability: thickness of 1.20 mm with specification of p = 800; zinc-nickel alloy electroplating, coating weights of zinc 17 - 24 g/m- minimum and if applicable chromium 40 - 70 mg/m^; chemical treatment of 0.5 -1.1 g/m-. maximum deviation from horizontal flat surface of 5 mm or more; with the camber of mother coils not larger than 2 mm per 2000 mm in length; having the following chemical composition (in percent by weight); carbon 0.005 maximum, silicon 1.0 - 1.6, manganese 0.6 maximum, phosphorus 0.13 maximum and sulfur 0.03 maximum; or (O) high strength electrolytic zinc-coated silicon steel flat-rolled products, whether or not including a chromate or chromate-free coating, with the following specifications: thickness 1.0 mm, thickness tolerance -t-/-50 p, width tolerance -0/+7 mm, tensile strength 45 - 49 kg/mm', yield point 32 - 36 kg/mm^ magnetic properties of permeability: thickness of '.00 mm with specification of p = 500; zinc-nickel alloy electroplating, coating weights of zinc 17 - 24 g/m' minimum.and if applicable chromium 45 - 75 mg/m';, maximum deviation from horizontal flat surface of 5 mm maximum; with the camber of mother coils not larger than 2 mm per 2000 mm in length; having the following chemical composition (in peicent by weight): carbon 0.005 maximum, silicon 1.0 - 1.6, manganese 0.6 maximum, phosphorus 0.15 maximum and sulfur 0.03 maximum; (xli) eleclrolytically tin-coated steel products, having differential coating with 22.4 g/m' box equivalent on the heavy side, with varied coating equivalents on the lighter side (as described below), with a continuous cast steel chemistry of type MR, with a surface finish of type 7B or 7C, with a surface passivation of 5.38 mg/m' of chromium applied as a cathodic dichromate treatment, with ultra flat scroll cut sheet form, with CAT 5 temper with 22.4/2.24 g/m^ coating, with a lithograph logo printed in a uniform pattern on the 2.24 g/m' coating side with a clear protective coat, with both sides waxed to a level of 108-144 mg/m", with ordered dimension combinations of (1) 0.208 mm thickness and 887.4 mm by 806.4 mm scroll cut dimensions; or (2) 0.208 mm thickness and 868.4

�